Metal-particle-induced enhancement of the photoluminescence from biomolecule-functionalized carbon nanotubes
© Kim et al.; licensee Springer. 2014
Received: 11 October 2013
Accepted: 7 February 2014
Published: 18 February 2014
The effect of metal particles on the photoluminescence (PL) and the Raman spectra of functionalized SWCNTs in aqueous solutions was systematically investigated by studying three different metal particles (gold, cobalt, and nickel) on three different SWCNT suspensions (DNA-, RNA-, and sodium deoxycholate salt (DOC)-functionalized SWCNTs). Substantial enhancement of the PL intensities was observed, while the Raman spectra remained unchanged, after gold, cobalt, or nickel particles were introduced into RNA-SWCNT aqueous suspensions. Almost the same results were obtained after the same metal particles were added to DNA-SWCNT aqueous suspensions. However, both the PL and the Raman spectra did not exhibit any change at all after the same metal particles were introduced into DOC-SWCNT aqueous suspensions. The unusual PL enhancements observed in this work cannot be accounted for by the three well-known mechanisms in the literature: surface-enhanced Raman scattering effect, Förster resonance energy transfer in a rebundling of isolated SWCNTs, and pH changes of the aqueous solutions.
KeywordsCarbon nanotube Metal-particle-induced photoluminescence enhancement RNA-functionalized carbon nanotube
Carbon nanotubes (CNTs) have been one of the most promising nanoscale materials for various applications due to their unique electrical, mechanical, thermal, and optical properties [1, 2]. Nevertheless, bundling of CNTs, due to their strong hydrophobicity, is an obstacle for many applications. For biological applications of CNTs, making stable aqueous suspension of individual CNTs by functionalizing their surface with appropriate biomolecules is essential [3, 4]. Single-stranded DNAs (ssDNAs) or double-stranded DNAs (dsDNAs) have been most commonly used for such functionalization of single-walled carbon nanotubes (SWCNTs), and optical properties of DNA-functionalized SWCNTs have been intensively studied [5–7].
Recently, SWCNT-based optical biosensors have been reported by several research groups [8–12]. Fluorescence bleaching of DAP-dex-functionalized SWCNTs when these complexes combine with nitric oxide was used for a nitric oxide (NO) sensor . An avidin sensor application was demonstrated by showing a fluorescence recovery when DLC-functionalized SWCNTs combined with avidin . The fluorescence quenching effect of insulin upon combining the insulin-binding-aptamer (IBA)-functionalized SWCNTs was used for an insulin detection . Biosensor application using fluorescence recovery when molecular-beacon-DNA-functionalized SWCNTs combined with the conjugate DNA or thrombin was reported . A Raman signal change of antibody-functionalized SWCNTs upon combining with corresponding bodies was demonstrated .
The optical property changes when metal ions or metal particles were introduced into a functionalized SWCNT suspension have also been extensively studied [13–18]. Photoluminescence (PL) enhancement of DNA-functionalized SWCNTs by terbium ions , fluorescence quenching of SDBS-functionalized SWCNTs by transition metal ions , fluorescence recovery of fluorophore-DNA-functionalized SWCNTs by silver ions and cysteine , and fluorescence quenching of GNQ-functionalized multi-walled carbon nanotubes (MWCNTs) by copper ions  were reported. Fluorescence quenching of PSMA-functionalized SWCNTs by gold nanoparticles of diameters of approximately 6 nm  was reported. But another study showed a Raman and fluorescence enhancement of SWCNTs by gold nanoparticles of diameters between 10 and 120 nm . In spite of many previous reports, the effect of metal ions and metal particles on the optical property of functionalized SWCNTs is yet to be further investigated. In order to systematically study the effect of metal particles on the optical property of functionalized SWCNTs, we tried three different metal particles (gold, cobalt, and nickel) on three different SWCNT suspensions (DNA-, RNA-, and sodium deoxycholate salt (DOC)-functionalized SWCNTs). We observed substantial enhancement of PL signals from SWCNTs by all three metal particles in both DNA-SWCNT suspension and RNA-SWCNT suspension, but no change in PL by any metal particle was observed in DOC-SWCNT suspension.
DNAs from herring sperm and DOC used in our work for functionalizing SWCNTs were purchased from Sigma-Aldrich (St. Louis, MO, USA). RNAs purified from Escherichia coli were obtained using the phenol extraction and ethanol precipitation method; and such as-purified total RNA dominantly consists of 2,904 (23S rRNA) and 1,542 (16S rRNA) nucleotides, corresponding to 990 and 480 nm in length, respectively. CoMoCAT SWCNTs were purchased from SouthWest Nanotechnologies Incorporated (Norman, OK, USA). The diameters of gold, cobalt, and nickel particles purchased from Alfa Aesar (Ward Hill, MA, USA) are 7.25 ± 1.75 μm, 1.40 ± 0.20 μm, and 5.00 ± 2.00 μm, respectively.
Aqueous suspensions of DNA-functionalized SWCNTs were prepared by adding SWCNTs (2.5 mg) to an aqueous DNA (0.68 mg/ml) solution of 25 ml, sonicating the solution using a bath-type sonicator (Branson 2510) for 2 h, and ultracentrifugation (T-1180; Kontron, Poway, CA, USA) at 50,000 × g for 1 h. Aqueous suspensions of RNA-functionalized SWCNTs were similarly prepared by adding SWCNTs (5 mg) to an aqueous RNA (1.4 mg/ml) solution of 50 ml, followed by the same sonication and centrifugation process. Aqueous suspensions of DOC-functionalized SWCNTs were prepared by adding SWCNTs (1 mg) to an aqueous DOC (2 wt.%) solution of 50 ml and sonicating the solution with a tip-type sonicator (Sonics Vibra cell VCX750; Sonics & Materials, Inc. Newtown, CT, USA) for 30 min, followed by the same centrifugation process.
Time-of-flight secondary ion mass spectrometry (TOF-SIMS) (TOF.SIMS5; ION-TOF, Heisenbergstr, Münster, Germany), with Bi+ as the primary ion source, was used to identify nucleotides in the synthesized DNA-SWCNT and RNA-SWCNT suspensions. PL and Raman spectra were measured at room temperature using 514 nm from an Ar+ laser (Innova 90C-6; Coherent Inc., Santa Clara, CA, USA) or 532-nm line from a frequency-doubled Nd:YAG laser (CL532-200-S; Crystalaser, Reno, Nevada, USA) as excitation light sources. Scattered light from the samples was analyzed through a single grating spectrometer (SP-2500i; Princeton Instruments, Trenton, NJ, USA) with a focal length of 50 cm and detected with a liquid-nitrogen-cooled silicon CCD detector (Princeton Instruments, Spec-10). A pH meter (Mettler Toledo, FE20; Thermo Fisher Scientific, Hudson, NH, USA) with glass electrodes was used to measure the pH of the solution samples.
In order to investigate the effect of metal particles on the PL and the Raman spectra, we carefully did as follows: 0.3 ml of the biomolecule-SWCNT suspension was put into a quartz cuvette, and PL and Raman spectra were taken right before 10 mg of each metal particle was added to the suspension; after a few minutes, most of the metal particles sedimented at the bottom of the cuvette; then PL and Raman spectra were taken at the exact same spot at 60, 120, and 180 min after the introduction of the metal particles.
Results and discussion
The atomic force microscopy (AFM) results (see Additional file 1) showed that the metal particles were not adsorbed on the SWCNTs. In fact, the size of the metal particles is a few micrometers whereas the diameter of the SWCNTs is approximately 1 nm. Thus, the metal particles are too big to be adsorbed on the SWCNTs. The metal particles just sedimented at the bottom of the cuvette and remained there during the optical measurements. Thus, the probed biomolecule-SWCNT suspension inside the laser spot was not directly in contact with the metal particles.
There are three well-known mechanisms for SWCNT PL enhancement. Surface-enhanced Raman scattering (SERS) effect is known to enhance PL intensities as well as Raman intensities via an amplified electric field near metal particles or a metal surface [21–23]. Since the Raman intensities of our sample did not show any enhancement at all, in spite of substantial PL enhancement, SERS effect cannot explain our PL enhancement results. PL enhancement, via Förster resonance energy transfer (FRET), was reported when a rebundling of isolated SWCNTs occurred, where the PL enhancement was accompanied by a peak red-shift or a suppression of high-energy PL peak intensity [20, 24–26]. There was no PL peak shift, and all the PL features were enhanced concurrently in our results. Thus, we can rule out FRET as the underlying mechanism of our PL enhancements. It is well known that pH has a strong effect on PL intensity of SWCNTs. At low pH environment, the surface oxidation of SWCNTs causes a PL bleaching, but the PL intensity recovers at high pH [27–29]. We have measured the pH change before and after the introduction of metal particles, and the measured pH increases were less than 0.3 for all three metal particles, Au, Co, and Ni, which is too small to induce any observable PL enhancement. Nonetheless, it is worthwhile to note that oxygen desorption from SWCNTs results in a PL enhancement . Thus, it would be reasonable to assert that oxygen desorption occurred for the biomolecule-functionalized SWCNTs upon the introduction of metal particles into the biomolecule-SWCNT suspension whereas it did not for the DOC-functionalized SWCNTs. Biomolecules such as DNA and RNA are structurally more flexible than the inorganic surfactant DOC. Subtle changes of the solution induced by metal particles, e.g., slight pH change, could make biomolecules highly susceptible to some structural change, which could lead to oxygen desorption from SWCNTs.
In summary, we have systematically investigated the effect of metal particles on the PL and the Raman spectra of functionalized SWCNTs in aqueous solutions. Substantial enhancement of the PL intensities was observed, while the Raman spectra remained unchanged, after gold, cobalt, or nickel particles were introduced into RNA-SWCNT aqueous suspensions. Almost the same results were obtained after the same metal particles were added to DNA-SWCNT aqueous suspensions. However, both the PL and the Raman spectra did not exhibit any change at all after the same metal particles were introduced into DOC-SWCNT aqueous suspensions. The unusual PL enhancements observed in this work cannot be accounted for by the three well-known mechanisms in the literature; SERS effect, FRET in a rebundling of isolated SWCNTs, and pH changes of the aqueous solutions. We suggest that oxygen desorption which occurred in the biomolecule-functionalized SWCNTs upon the introduction of metal particles be responsible for the observed PL enhancement.
sodium deoxycholate salt
single-walled carbon nanotube
time-of-flight secondary ion mass spectrometry.
This research was supported by Basic Science Research Program through the National Research Foundation of Korea (NRF) funded by the Ministry of Education (2009–0093817 and 2013R1A1A2010595). SH acknowledges the support from the NRF grant (H-GUARD 2013M3A6B2078961).
- Iijima S: Helical microtubules of graphitic carbon. Nature 1991, 354: 56–58. 10.1038/354056a0View ArticleGoogle Scholar
- Dresselhaus G, Dresselhaus MS, Avouris P: Carbon Nanotubes: Synthesis, Structure, Properties and Applications. Berlin: Springer; 2001.View ArticleGoogle Scholar
- Meng L, Fu C, Lu Q: Advanced technology for functionalization of carbon nanotubes. Prog Nat Sci 2009, 19: 801–810. 10.1016/j.pnsc.2008.08.011View ArticleGoogle Scholar
- Nakashima N: Soluble carbon nanotubes: fundamentals and applications. Int J Nanosci 2005, 4: 119–137. 10.1142/S0219581X05002985View ArticleGoogle Scholar
- Zheng M, Jagota A, Strano MS, Santos AP, Barone P, Chou SG, Diner BA, Dresselhaus MS, Mclean RS, Onoa GB, Samsonidze GG, Semke ED, Usrey M, Walls DJ: Structure-based carbon nanotubes sorting by sequence-dependent DNA assembly. Science 2003, 302: 1545–1548. 10.1126/science.1091911View ArticleGoogle Scholar
- Zheng M, Jagota A, Semke ED, Diner BA, Mclean RS, Lustig SR, Richardson RE, Tassi NG: DNA-assisted dispersion and separation of carbon nanotubes. Nat Mater 2003, 2: 338–342. 10.1038/nmat877View ArticleGoogle Scholar
- Nakashima N, Okuzono S, Murakami H, Nakai T, Yoshikawa K: DNA dissolves single-walled carbon nanotubes in water. Chem Lett 2003, 32: 456–457. 10.1246/cl.2003.456View ArticleGoogle Scholar
- Kim JH, Heller DA, Barone PW, Song C, Zhang J, Trudel LJ, Wogan GN, Tannenbaum SR, Strano MS: The rational design of nitric oxide selectivity in single-walled carbon nanotubes near-infrared fluorescence sensors for biological detection. Nat Chem 2009, 1: 473–481. 10.1038/nchem.332View ArticleGoogle Scholar
- Satishkumar BC, Brown LO, Gao Y, Wang C-C, Wang H-L, Doorn SK: Reversible fluorescence quenching in carbon nanotubes for biomolecular sensing. Nat Nanotechnol 2007, 2: 560–564. 10.1038/nnano.2007.261View ArticleGoogle Scholar
- Cha T-G, Baker BA, Sauffer MD, Salgago J, Jaroch D, Rickus JL, Porterfield DM, Choi JH: Optical nanosensor architecture for cell-signaling molecules using DNA aptamer-coated carbon nanotubes. ACS Nano 2011, 5: 4236–4244. 10.1021/nn201323hView ArticleGoogle Scholar
- Yang R, Tang Z, Yan J, Kang H, Kim Y, Zhu Z, Tan W: Noncovalent assembly of carbon nanotubes and single-stranded DNA: an effective sensing platform for probing biomolecular interactions. Anal Chem 2008, 80: 7408–7413. 10.1021/ac801118pView ArticleGoogle Scholar
- Chen Z, Tabakman SM, Goodwin AP, Kattah MG, Daranciang D, Wang X, Zhang X, Liu Z, Utz PJ, Jiang K, Fan S, Dai H: Protein microarrays with carbon nanotubes as multicolor Raman labels. Nat Biotechnol 2008, 26: 1285–1292. 10.1038/nbt.1501View ArticleGoogle Scholar
- Ignatova T, Najafov H, Ryasnyansky A, Biaggio I, Zheng M, Rotkin SV: Significant FRET between SWNT/DNA and rare earth ions: a signature of their spatial correlations. ACS Nano 2011, 5: 6052–6059. 10.1021/nn201911bView ArticleGoogle Scholar
- Brege JJ, Gallaway C, Barron AR: Fluorescence quenching of single-walled carbon nanotubes with transition-metal ions. J Phys Chem C 2009, 113: 4270–4276. 10.1021/jp808667bView ArticleGoogle Scholar
- Zhao C, Qu K, Song Y, Xu C, Ren J, Qu X: A reusable DNA single-walled carbon-nanotube-based fluorescent sensor for high sensitive and selective detection of Ag+ and cysteine in aqueous solutions. Chem Eur J 2010, 16: 8147–8154. 10.1002/chem.201000306View ArticleGoogle Scholar
- Dong Z, Jin J, Zhao W, Geng H, Zhao P, Li R, Ma J: Quinoline group grafted carbon nanotube fluorescent sensor for detection of Cu2+ ion. Appl Surf Sci 2009, 255: 9526–9530. 10.1016/j.apsusc.2009.07.089View ArticleGoogle Scholar
- Wang D, Li Z-C, Chen L: Templated synthesis of single-walled carbon nanotube and metal nanoparticle assemblies in solution. J Am Chem Soc 2006, 128: 15078–15079. 10.1021/ja066617jView ArticleGoogle Scholar
- Scolari M, Mews A, Fu N, Myalitsin A, Assmus T, Balasubramanian K, Burghard M, Kern K: Surface enhanced Raman scattering of carbon nanotubes decorated by individual fluorescent gold particles. J Phys Chem C 2008, 112: 391–396. 10.1021/jp076190iView ArticleGoogle Scholar
- Lee C-Y, Harbers GM, Grainger DW, Gamble LJ, Castner DG: Fluorescence, XPS, and TOF-SIMS surface chemical state image analysis of DNA microarrays. J Am Chem Soc 2007, 129: 9429–9438. 10.1021/ja071879mView ArticleGoogle Scholar
- Tan PH, Rozhin AG, Hasan T, Hu P, Scardaci V, Milne WI, Ferrari AC: Photoluminescence spectroscopy of carbon nanotube bundles: evidence for exciton energy transfer. Phys Rev Lett 2007, 99(137402):1–4.Google Scholar
- Schats GC, Young MA, Van Duyne RP: Electromagnetic mechanism of SERS. Top Appl Phys 2006, 103: 19–46. 10.1007/3-540-33567-6_2View ArticleGoogle Scholar
- Tabakman SM, Chen Z, Casalongue HS, Wang H, Dai H: A new approach to solution phase gold seeding for SERS substrates. Small 2011, 7: 499–505. 10.1002/smll.201001836View ArticleGoogle Scholar
- Hong G, Tabakman SM, Welsher K, Wang H, Wang X, Dai H: Metal-enhanced fluorescence of carbon nanotubes. J Am Chem Soc 2010, 132: 15920–15923. 10.1021/ja1087997View ArticleGoogle Scholar
- Lefebvre J, Finnie P: Photoluminescence and Förster resonance energy transfer in elemental bundles of single-walled carbon nanotubes. J Phys Chem C 2009, 113: 7536–7540. 10.1021/jp810892zView ArticleGoogle Scholar
- Yang J, Yang N, Zhang D, Wang X, Li Y, Li Y: Photoluminescence from exciton energy transfer of single-walled carbon nanotube bundles dispersed in ionic liquids. J Phys Chem C 2012, 116: 22028–22035. 10.1021/jp306515aView ArticleGoogle Scholar
- Torrens ON, Milkie DE, Zheng M, Kikkawa JM: Photoluminescence from intertube carrier migration in single-walled carbon nanotube bundles. Nano Lett 2006, 6: 2864–2867. 10.1021/nl062071nView ArticleGoogle Scholar
- Karachevtsev VA, Glamazda AY, Plokhotnichenko AM, Leontiev VS, Linnik AS: Comparative study on protection properties of anionic surfactants (SDS, SDBS) and DNA covering of single-walled carbon nanotubes against pH influence: luminescence and absorption spectroscopy study. Mat-Wiss U Werkstofftech 2011, 42: 41–46. 10.1002/mawe.201100728View ArticleGoogle Scholar
- Noguchi Y, Fujigaya T, Niidome Y, Nakashima N: Regulation of the near-IR spectral properties of individually dissolved single-walled carbon nanotubes in aqueous solutions of dsDNA. Chem Eur J 2008, 14: 5966–5973. 10.1002/chem.200800070View ArticleGoogle Scholar
- Dukovic G, White BE, Zhou Z, Wang F, Jockusch S, Steigerwald ML, Heinz TF, Friesner RA, Turro NJ, Brus LE: Reversible surface oxidation and efficient luminescence quenching in semiconductor single-walled carbon nanotubes. J Am Chem Soc 2004, 125: 15269–15276.View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.